Little data is available about the material properties and swelling response of the elsatomers used in swell packers. This information is necessary for modeling and simulation of these elastomers in different petroleum applications. An experimental setup was therefore designed and implemented at Sultan Qaboos University (SQU) to investigate the material behavior of these elastomers under tension and compression, so that these properties could be used for different simulations. Before developing a finite element model (FEM) of elastomer seal performance, it was felt that a thorough evaluation needs to be carried out to decide which of the currently available material models is most suitable for swelling elastomers. This comparison translates into the selection of the correct strain energy function for accurate determination of material coefficients. Different hyperelastic material models are compared here. Experimental investigations under tensile and compressive loads, along with their numerical analysis are presented in detail in this chapter.
- Swelling elastomer
- finite element simulation
- material model
- model comparison
Metallic and rubber seals have been used for quite some time in oilfield development. However, the advent of swelling elastomer seals has revolutionized the technology. Deployment of swelling elastomers in a variety of petroleum applications are discussed in detail in Chapter 2. Before using swelling elastomers for any application, behavior under different fluids and environmental conditions should be known to predict the actual response. It can be done experimentally, analytically, or through numerical simulations. Though it would be most efficient time-wise, no analytical work is available that entirely explains the behavior of these materials. On the other hand, it is difficult, costly, and time-consuming (and at times even impossible) to perform experiments for all the possible conditions. Hence, a robust numerical simulation strategy, validated against experimental results, can be used to predict the behavior of swelling elastomers.
Little data is available (about their material properties and swelling response), which is needed for modeling and simulation of these elastomers in different petroleum applications. An experimental setup was therefore designed and implemented at Sultan Qaboos University (SQU) to investigate the material behavior of these elastomers under tension and compression, so that these properties could be used for different simulations. Before developing a finite element model (FEM) of elastomer seal performance, it was felt that a thorough evaluation needs to be carried out to decide which of the currently available material models is most suitable for swelling elastomers. This comparison translates into the selection of the correct strain energy function for accurate determination of material coefficients. Different hyperelastic material models are compared here. Experimental investigations under tensile and compressive loads, along with their numerical analysis are presented in detail in this chapter.
2. Models for rubberlike materials
Rubber elasticity theory explains the mechanical properties of a rubber in terms of its molecular constitution. This approach involves two essentially separate issues. First is the treatment of the statistical properties of a single long-chain molecule in terms of its geometrical structure. Second comes the application of this treatment to the problem of the network of long-chain molecules corresponding to a cross-linked or vulcanized rubber.
First statistical mechanics approach to describe the force on a deforming elastomer network was based on Gaussian statistics. The basic assumption in this theory is that a chain never approaches its fully extended length. The problem was initially attempted by Kuhn and Grun  who derived a relation between elastic modulus and molecular weight. More precise treatment leading to explicit forms of stress–strain curves valid for large strains were developed by Wall , Flory and Rehner [3, 4]
, and, James and Guth . Results show that these models fail to capture large and even moderate stretches. Hence many constitutive models were developed in an attempt to predict the behavior not only for small stretch levels but also for medium and large stretches.
Other researchers followed non-Gaussian statistics. These are physical models based on an explanation of a molecular chain network, phenomenological invariant-based and stretch-based continuum mechanics approach. The distinctive feature of non-Gaussian approach is that it presumes that a chain can attain its fully extended length. Phenomenological approach is used to relate empirical findings of certain phenomena in such a way that it is consistent with fundamental theory, but is not directly derived from theory. This approach is further divided into stretch-based and invariant-based models. Invariants are basically defined by principal stretches. Models in which stretches can be written in terms of invariants are classified as invariant-based models, while models that cannot be converted into invariants are known as stretch-based models. Micromechanical models describe a material as a three-dimensional network and consider statistical mechanics arguments on networks of cross-linked long-chain molecules. A hyperelastic material model is a type of constitutive relation for rubberlike materials in which the stress–strain relationship is developed from a function. Most continuum mechanics treatment of rubber elasticity begins with assuming rubbers to be hyperelastic and isotropic in nature. Figure 1 gives a broad classification of different types of hyperelastic material models.
2.1 Micromechanical models
These models assume a unit cell which deforms in a principal-stretch space to relate individual chain stretch to applied deformation. Wang and Guth  proposed a three-chain model in which chains are located along the axes of cube. The chains deform affinely with the cell, and stretch of each chain corresponds to the principal stretch value. The strain energy function is given by
Here, is the inverse Langevin,
Arruda and Boyce  proposed an eight-chain model in which chains align along diagonals of a unit cell. Due to the symmetry of chain structure, the interior junction point remains at the center throughout the deformation. Strain energy function is given by
Wu and Giessen  suggested a full network chain model in which chains are randomly distributed and deform in an affine manner. Strain energy response is determined by overall integration which is computationally intensive; expression for strain energy is therefore reproduced here. To develop constitutive relations, work done by the stresses is established in terms of strain energy function. Strain energy function must depend on the amount of stretch via invariants of the stretch tensor. The coefficients in these functions should be determined by uniaxial, biaxial, and shear test data. The essential problem is to determine the strain energy function for providing good fit with a number of sets of experimental data.
2.2 Phenomenological invariant-based models
One of the first attempts at a hyperelastic material model based on the phenomenological invariant-based approach was made independently by the two scientists Mooney  and Rivlin . Due to the assumption of incompressibility, the third invariant is not considered, yielding the following expression for strain energy function:
By keeping only the second term of this expression, we get the famous Mooney-Rivlin model for elastomer deformation
Mooney-Rivlin model makes passable predictions for uniaxial and shear cases in the low-stretch region, but does not yield good predictions for equibiaxial case and uniaxial and shear cases in the large-stretch region. As reported by Treloar  and Boyce and Arruda , when only the first term of Mooney-Rivlin strain energy function is retained, it becomes the neo-Hookean model:
Kilian  explains that van der Waal hyperelastic material model gives the mathematical relation in terms of the initial shear stress ‘
Gent  proposed a new constitutive relation for strain energy function which is given by the expression
where , and is the maximum value for .
The Yeoh model  is derived from Rivlin strain energy function by expanding only the first three terms, and neglecting the second invariant, yielding:
The Marlow hyperelastic material model  is another variation of this approach:
2.3 Phenomenological stretch-based models
Ogden model  proposes a strain energy function based on the principal stretches for incompressible materials. Principal stretches are directly measurable quantities and it is one obvious advantage of using them. Ogden strain energy function is given by
where and are material constants. Nonlinear least square optimization technique is used by Twizell and Ogden  to determine the stable constants for the above strain energy function and to find an improve fit to the data when ‘
There are various other forms of strain energy potentials (Figure 1) for modeling hyperelastic isotropic elastomers, such as the ones reported by Ali et al. , Hossain and Steinmann , and Steinmann et al. . However, these functions seldom describe the complete behavior of these swellable materials, especially for different loading conditions.
2.4 Other models
Some researchers have attempted to develop material models which explain the stress-stretch behavior of an elastomer after swelling to a particular level. As described by Treloar , Gauss model follows a molecular approach and involves swelling ratio ‘’:
Increasing discrepancies between Gaussian theory and experiments have been recognized when moving from small to large stretch levels. This discrepancy is amplified when the effect of swelling is included. Flory and Erman  model predicts the swelling behavior reasonably well only for small to moderate stretches. Arruda-Boyce model (for stress-stretch behavior coupled with elastomer swelling) is based on a simplified representation of eight chains lying along the diagonal of a cubic cell. The Cauchy stress for Arruda-Boyce model  is given by the following relation:
This model, when used for predicting swelling behavior of elastomers, gives close results only for large stretch. They later attempted to combine their model with Flory-Erman model. This hybrid model is supposed to take into account the actual effect of swelling for small to large stretches. However, even this hybrid model fails to replicate the actual behavior of swelling elastomers.
A few models have been proposed by authors such as Wagner . These are basically hyperelastic models that also include swelling ratio, but fail to give reasonable predictions. There is hence a need for a model that predicts the actual behavior, and includes factors such as energy of mixing, and effect of diffusion, together with hyperelastic effect.
2.5 Energy-diffusion models
Other authors have suggested more realistic constitutive models for elastomers subjected to swelling, in which changes due to configuration entropy are considered along with energy of mixing and diffusion. According to Flory-Rehner theory [3, 4], free energy density can be written as the sum of strain energy density function due to thermodynamics of mixing and configuration entropy of polymer network. A number of authors use this concept to develop a relation for the prediction of swelling, such as Han et al. , Cai and Suo , Chester and Anand , Drozdov and Christiansen , Hong et al. , and Lucantonio et al. .
Flory-Huggins theory, proposed by Flory  and Huggins , considers the changes in entropy due to mixing. Changes due to configuration entropy are added by considering different available hyperelastic material models as discussed above. As explained by Lucantonio , Hong et al. , and Kang and Huang , solvent influx in swelling elastomer follows the diffusion phenomenon. A few authors, such as Biot , Cai et al. , Lucantonio and Nardinocchi , and Tomari and Doi , use the concept of porous media and assume swelling elastomer or gel to be poro-elastic. A porous material is made up of pores and its permeability is related to the pore size. Major portion of a swollen elastomer contains solvent which resists when under the influence of force. That is why models based on poro-elastic concept do not predict good swelling results in general as discussed by Hong et al. .
Most of the chemo-mechanical models use Gaussian-chain model for mechanical configuration changes that consider small stretching of chains, and use Fick’s law to define fluid influx. Again, they give reasonable results only at small swelling levels. Material models for predicting swelling in polymer networks are discussed below.
2.5.1 Poroelastic models
Biot  used Darcy’s law along with thermodynamics of mixing to model fluid influx into a porous medium (soil), the approach being known as poro-elasticity theory. This theory is used in a variety of applications to study porous materials from soils to tissues. Tomari and Doi  used the concept of poro-elasticity to develop a model for swelling dynamics. They assumed swelling time to be proportional to gel size, frictional constant, and changes in stresses. Barrière and Leibler  proposed a swelling model that is based on a porous media concept and includes frictional effect between elastomer and fluid. To describe fluid influx they use the dependence of coefficient of diffusion on concentration, and do not use Fick’s law (as according to them it does not predict good behavior at large swelling). Cai et al.  performed experiments on swollen gel that is compressed between two plates. They developed a model using linear poro-elasticity for the experiments performed. Variational approach is employed by Baek and Pence  to investigate gels in equilibrium, subjected to loading on surface. They do not take into account the relationship for dynamical processes (like diffusion) prior to equilibrium. Lucantonio and Nardinocchi  describe bending due to swelling in a gel considering poro-elastic linear theory. Lucantonio et al.  investigated the stability between linear poro-elastic and nonlinear theory approaches assuming Gaussian statistics and homogenous configuration. Instead of considering dry state as reference configuration (like other models), they assume initially swollen elastomer as a reference state. Constitutive relations are derived using weak-form variational formulation. Bouklas and Huang  present a comparison of linear poro-elasticity and nonlinear Gaussian based (chemo-mechanical) theories. Both theories give similar results at small swelling ratios, but for higher swelling ratios linear theory fails and gives large errors as compared to nonlinear theory.
2.5.2 Chemo-mechanical models
Durning and Morman  use phantom network model along with Bastide’s scaling model for taking into account the entropy changes due to configuration. Fick’s law is used for describing fluid influx. Inconsistencies are present due to the use of Fick’s law, as it does not provide a solution for nonlocal effects. Chemo-mechanical theory for hydrogels was developed by Dolbow et al.  and extended finite element method was implemented to study swelling. Continuum based sharp interface model and swelling kinetics for temperature sensitive stimulus responsive hydrogels was developed by Ji et al. . Hong et al.  assume short and long range migration of solvent inside the polymer. Developed theory is based on non-equilibrium thermodynamics and considers free energy and kinetics to be material specific. They use Flory-Huggins theory to describe changes in free energy, while Gaussian approach is used for defining changes in entropy due to network configuration. They use the diffusion equation for fluid inflow of Feynman et al. , in which flux is proportional to gradient of chemical potential. Hong et al.  developed an equilibrium theory using Gibb’s approach. Legendre transformation is used to represent the field in gel, analogous to compressible hyperelastic solid. Developed model is used on kinetics of fluid influx and Gaussian approach. User-defined subroutine (UHYPER) in ABAQUS is also developed for the model. Duda et al.  follow Gibb’s idea of multi-component solid for the development of an expression for swelling equilibrium. Theory is based on mechanics (macro) and chemistry (micro) of mixing of solid and fluid. They consider Gaussian neo-Hookean model for changes in configuration entropy of the elastomer. Development of the model assumes that the body is not fully immersed into the fluid. Kang and Huang  formulated a model based on variational approach to set governing equations combining chemical and mechanical conditions. They used similar approach as Hong et al. , following Gaussian-chain model for configuration entropy and Flory-Huggins equation for energy of mixing. They also develop an explicit formulation for tangent modulus and true stress. User-defined subroutine (UMAT) in ABAQUS is also developed for numerical investigation and comparison is done with user subroutine developed by Hong et al. .
A continuum mechanical theory along with fluid imbibition was developed by Chester and Anand . They first use Gaussian approach to develop a model for swelling phenomenon. Fluid influx is taken into account using Darcy’s law. Then they use micro mechanical non-Gaussian based approach for model improvement. As a further extension to their work, they include thermal effect and develop coupled equation for stretching, fluid influx, and heat transfer. Cai and Suo  use Flory-Rehner model to describe the changes in entropy due to stretching, but ignore the changes in entropy due to mixing of fluid and polymer. They develop an equation of state based on Gaussian-chain model considering stretching only. Yan and Jin  take into account the entanglements of chains, by using hybrid free energy function based on Edwards-Vilgis slip-link model and Flory-Huggins theory. Drozdov and Christiansen  propose a swelling model based on viscoelasticity and viscoplasticity. They study hydrogels, under both tensile and compressive loads, to investigate the effect of strain rate on elastic properties. Constitutive relations are based on viscoelasticity of gels.
All of the above models generally give reasonable results only for small swelling. For large swelling (as in the case of swelling elastomers), most of these models do not give close approximation to actual data.
3. Material models for swelling elastomers
None of the existing material models accurately represent the behavior of swelling elastomers. Different types of models for rubberlike materials were briefly described above. Major material models that can be used to represent stretchable elastomers, though not very accurately, are discussed in more detail in this section. As mentioned above, a swelling elastomer can be treated as a hyperelastic material, commonly modeled as an incompressible, homogeneous, isotropic, and nonlinear elastic solid. Due to its long and flexible structure, an elastomer has the ability to stretch to several times its initial length. Elastomers at small strains (up to 10%) have linear stress strain relation, and behave like other elastic materials . In case of applications where large deformations exist, theory of large elastic deformation should be considered. Several theories for large elastic deformation have been developed for hyperelastic materials based on strain energy density functions. These models are based on phenomenological based continuum mechanics approach and micromechanically motivated network approach [20, 21]. Phenomenological models contain invariant-based or principal stretch-based approach usually containing polynomial functions. Micromechanical models typically have terms for cross-linked long-chain molecules [3, 4, 6, 8, 50]. Selection of appropriate strain energy potentials and correct determination of material coefficients are the main factors for modeling and simulation.
3.1 Gaussian Hyperelastic material models
One major approach used to define the deformations in elastomer chains follows Gaussian statistics, Neo-Hookean model being a good example. In Gaussian statistics, a chain never approaches the maximum stretch; rather, it is limited to small-to-moderate stretches. For a three dimensional polymer, due to its large chain density, probability distribution for any event
Standard deviation in terms of chain density () and distance between the chain ends () is given by Treloar  as
and assigning , we get the following relation
Taking summation for all chains, substituting into Eq. (17), and on simplification we get
Shear modulus for rubbers and elastomers is given by G=. Helmholtz free energy is given by , hence Eq. (18) can be written as
where is the first invariant of stretch. Eq. (19) gives the strain energy function for neo-Hookean model [13, 23]. As it is derived using Gaussian statistics, it gives linear response for material where elastomer chain undergoes only small to moderate stretches.
3.2 Non-Gaussian Hyperelastic material models
Hyperelastic material models that follow non-Gaussian statistics consider that chains can stretch to reach maximum extensibility. Many models are formulated based on this approach, such as Mooney-Rivlin , Yeoh , Arruda-Boyce , Ogden , Gent , etc. Mooney-Rivlin model follows Valanis and Landel theory  according to which strain energy function for an isotropic material in finite deformation is of the form
Invariants based on principal stretches are given by
For an incompressible isotropic material, third invariant vanishes and strain energy becomes a function of and only:
Eq. (22) gives the strain energy function for Mooney-Rivlin model, where and are material constants. According to this theory, stress–strain behavior depends upon the partial derivatives . Characterization of elastic properties of a polymer consists of determining these partial differentials through experimental measurements. These partial differentials cannot be determined from experiments with only one deformation mode. Preferred methods are generally biaxial extension where stretches in both directions vary independently. Yeoh assumed that is much larger than , so the second partial derivative can be neglected. Strain energy function for Rivlin  can then be written as
where index ‘’ will always be zero. If the series is truncated after three terms, we get the expression for strain energy function for Yeoh model :
where , and are material coefficients determined by fitting experimental data. If Eq. (23) is expanded only for ‘’, we get the Neo-Hookean strain energy function, in which .
Another stretch based non-Gaussian phenomenological strain energy function for hyperelastic materials was proposed by Ogden . This model is given by the following relation in terms of principal stretches:
Here, ‘’ and ‘’ are material constants that are determined by fitting the experimental data, and ‘’ is a positive definite integer. Material constants are related to shear modulus () by the following relation:
Second degree Ogden strain energy function is given by expanding Eq. (24) for ‘’:
It is interesting to note that if Ogden model Eq. (24) is expanded for ‘’ and for , , it gives an expression similar to the Mooney-Rivlin model:
Also, if Ogden model is expanded for ‘’ with , , it reduces to the neo-Hooken model:
Arruda-Boyce model  uses the statistical mechanics approach followed by many researchers [3, 4, 6, 50]. Instead of the 3-chain  and 4-chain models [3, 4] of earlier researchers, Arruda-Boyce proposed a more accurate 8-chain approach, yielding the following strain energy function:
Here, is the inverse Langevin, is the chain density, is the Boltzman constant, is the temperature, is the chain length, and is the chain stretch. Also, is the effective shear modulus.
Since , and , we can get
By showing that the expression for chain stretch reduces to a function of the first stretch invariant, , and using Eqs. 4.30 and 4.31, the final expression for Arruda-Boyce strain energy function becomes
Gent  proposed an empirical constitutive relation using only two constants for the entire range of strains for hyperelastic materials. In statistical mechanics approach, when a chain reaches the fully stretched state, it is known as locking stretch. Gent describes this stretch as a maximum value of denoted by , so that the strain energy function is given by the following relation:
Boyce  performed a comparison between Gent and Arruda-Boyce eight chain models. As and , Gent model can be expanded using natural logarithm.
Similarly, Arruda-Boyce model can be re-written in terms of general invariant based form as follows
Eqs. 4.34 and 4.35 can be used to predict large stretch deformations.
There are many hyperelastic material models available. Some of them are presented in this section, while others were discussed in the previous section. Models such as Van der Waal and Marlow models have not been presented here because they do not show good convergence for swelling elastomers. Next section gives the comparison of different hyperelastic material models against experimental results from uniaxial tensile tests.
4. Comparison of material models under tensile loading
As none of the available material models accurately represents swelling elastomers, modeling of these elastomers based on current models can yield only approximate results. Before this, no evaluation of material models for prediction of swelling elastomer behavior could be found in published literature. This study was therefore conducted to have a comparative assessment of current hyperelastic material models; how closely they predict the actual behavior under tension. Two water swelling elastomers are used for experimental and numerical investigation under tension (material-
4.1 Experimental work
The main objective of the experimental work is to provide actual tensile test data to extract parameters for the material models, and then to compare predicted behavior from each model against the actual tensile behavior. A large number of samples of two different water-swelling elastomers were allowed to swell for 8 days in saline water of 40,000 ppm (4%) concentration at a temperature of 60°C (actual field conditions in a regional oil-well). Tensile tests were carried out on ring samples before and after swelling, reported values being average of readings from three samples. As expected, the material expands due to swelling. Dimensions of the ring samples before and after swelling are shown in Figure 2.
4.1.1 Sample preparation
Ring samples were cut in line with ASTM-D412, using a die-and-punch set; outside diameter (
4.1.2 Test procedure
Width, thickness, and flattened length of all ring samples (before and after swelling) are recorded prior to conducting the tensile test, to be used later for stress and strain measurements. Specially fabricated (in-house) hook-type fixtures (in accordance with ASTM D412) are used to grip the ring samples. A small pre-tension is applied on each sample to get the flattened length as shown in Figure 3. A loading rate of 500 mm/min is used until the sample ruptures. Force-elongation and stress–strain readings are automatically recorded by the machine.
4.2 Numerical Modeling and simulation
Tensile tests are modeled and simulated using the commercial finite element package ABAQUS. Standard dumbbell shaped tensile specimen is used for simulation because of its symmetric nature, allowing modeling of only one-quarter of the sample; Figure 4. Load application is also simplified because of this sample geometry, yielding proper uni-axial tension. Swelling elastomer specimen is modeled as a hyperelastic body using 8-noded linear brick element with reduced integration (C3D8R). Deformed specimen is also shown in Figure 4. Minor inconsistencies between experimental and simulated results can be expected, as the sample geometries (ring-type and dumbbell-type) are different.
Four well-known material models (Ogden, Yeoh, Arruda-Boyce, and neo-Hookean) are selected from the pool of hyperelastic models available in ABAQUS. These are known to show convergence and good agreement with experimental data for elastomeric materials under tension. Coefficients for each model are extracted from the uniaxial tensile test data (experimental) using curve fitting techniques. Poisson’s ratio for these elastomers has been taken as υ = 0.495, while density values (from actual experiments) for un-swelled (US) and swelled (S) specimens of materials
4.3 Results and discussion
For both materials, finite element simulation of uni-axial tensile test is done using the four most popular material models for the un-swelled and 8-day swelled conditions. Stress–strain curves from simulations, using the selected material models, are compared with experimental results. Results are plotted separately for materials
Figure 5 shows comparison of stress–strain curves for experimental and FE simulation data for un-swelled and swelled (8 days) conditions for material
Based on results of the current study, the neo-Hookean model appears to be the best suited for both un-swelled and swelled (small to medium stretch) conditions under tensile loads, but it starts diverging away from experimental results for very large strains. For large strains (which is the case in real-world use of swelling elastomer seals), Ogden model is consistently better than the others. However, it can be seen that no material model predicts results close to the experimental values. The reason might be that energy and diffusion effects are not considered in these models.
5. Comparison of material models under compressive loading
Petroleum industry uses swelling elastomers in a variety of applications as discussed in detail in Chapter 2. Being primarily used as a sealing element, swelling elastomers generally experience compressive loads. Hence, investigation of such elastomers under compression is very important. A comparison of currently available hyperelastic material models is presented in this section against experimental results for two swelling elastomers (
5.1 Experimental work
To replicate actual field conditions in many regional oil wells, Qamar et al. [56, 57] used samples of two types of water-swelling elastomers in various petroleum development applications were subjected to swelling in saline water of 0.6% (6,000 ppm) and 12% (120,000 ppm) concentrations maintained at a temperature of 50°C. To investigate the effect of swelling, samples were taken out for mechanical testing after 1, 2, 4, 7, 10, 16, 23, and 30 days of swelling. The elastomers were of a fast-swell type, so readings were initially taken after almost each day, and on a weekly basis later on.
5.1.1 Sample preparation
Disc samples were cut using a die-and-punch set, with some surface grinding needed for final trimming. As prescribed by ASTM-D575, disc dimensions for compression testing are 28.5 mm diameter and 12.5 mm thickness. Due to reasons of confidentiality, actual identification number of swelling-elastomer materials is not mentioned here.
5.1.2 Test procedure
Compression tests are performed on a Tinius Olsen universal testing machine in the compression mode, using a 50-kN load cell; Figure 7. Disc specimen is placed on a fixed bottom plate while the top plate applies a compressive load on the specimen. Elastomer sample is free to expand in the radial direction. Top surface of the disc moves downward with the compression load, while bottom surface is not allowed to move in the axial direction. Load is applied at a rate of 12 mm/min (ASTM-D575) until the specimen thickness is compressed to 10 mm. Force-deformation and stress–strain data are recorded. A small barreling effect can be observed in the compressed sample.
5.2 Numerical Modeling and simulation
Finite element analysis for predicting the deformation behavior of swelling elastomers under compression for both the materials in two salinities solutions are performed using commercial finite element analysis package ABAQUS . Swelling elastomer specimen is modeled using 8-noded linear brick element with reduced integration (C3D8R). Stress–strain data obtained from experiments are used to extract coefficients that define the constitutive relation in finite element analysis. Material parameters such as Poisson’s ratio and density at each condition with swelling for different days are also determined experimentally. ASTM standard disc geometry is modeled for simulation of compression tests. Compressive loads and boundary conditions are in line with experimental values. Simulations are conducted before swelling and after each swelling period for a total of one month period under both salinities. Figure 8 shows the deformed and undeformed specimens.
5.3 Results and discussion
Finite element simulations of compression experiments are carried out for comparison of the five most suitable hyperelastic material models, including Ogden model with both first and second strain energy functions. Stress–strain curves obtained through simulations (for both the materials) are compared against experimental results after each swelling period.
Experimental and numerical stress–strain curves are compared in Figure 9, for material
Experimental stress–strain curves for material
Experimental investigation of performance of swelling elastomer seals (such as sealing pressure at various stages of swelling) is highly difficult and very costly. Numerical simulations, if yielding reasonable predictions, can be a much better alternative. If we want to conduct numerical studies of elastomer seal performance, Ogden model with second-degree strain energy function will have to be used as it gives overall best results both under tensile and compressive loads. This best available current hyperelastic model (Ogden-2) has been later used to study the mechanical and structural behavior of swelling elastomers under compressive loading in Chapter 7, and to evaluate the performance of swelling elastomer seals in Chapter 8.
To more accurately predict the behavior of swelling elastomers, thermodynamics of mixing and the phenomenon of diffusion should also be considered. Starting with the Ogden model, this approach for mechanics of swelling is followed in Chapter-6 to develop a new material model for swelling elastomers.
Simulations have been carried out to compare different hyperelastic material models against experimental results for swelling elastomers subjected to tensile and compressive loading, including Arruda-Boyce, Ogden (N = 1), Ogden (N = 2), Yeoh, and neo-Hookean models. Following ASTM standards, experiments were conducted on ring samples (for tensile tests) and disc samples (for compression tests), before swelling, and after 8 days of swelling, using two swelling elastomer materials. Simulations were performed using the FEA package ABAQUS. For tensile loads, most of the models give reasonable predictions for small deformations. For medium to large deformations, Ogden model with second strain energy function (Ogden-2) gives best results. For simulations under compression, many models do not give good predictions even for small loads. Ogden-2 again yields overall minimum error. Hyperelastic models can be used for FE analysis of swellables, giving reasonably acceptable approximations. However, a new material model is definitely needed to capture the material behavior of swelling elastomers more accurately.